#### Read Topological insulators in Bi2Se3, Bi2Te3 and Sb2Te3 with a single Dirac cone on the surface text version

ARTICLES

PUBLISHED ONLINE: 10 MAY 2009 | DOI: 10.1038/NPHYS1270

Topological insulators in Bi2Se3, Bi2Te3 and Sb2Te3 with a single Dirac cone on the surface

Haijun Zhang1 , Chao-Xing Liu2 , Xiao-Liang Qi3 , Xi Dai1 , Zhong Fang1 and Shou-Cheng Zhang3 *

Topological insulators are new states of quantum matter in which surface states residing in the bulk insulating gap of such systems are protected by time-reversal symmetry. The study of such states was originally inspired by the robustness to scattering of conducting edge states in quantum Hall systems. Recently, such analogies have resulted in the discovery of topologically protected states in two-dimensional and three-dimensional band insulators with large spinorbit coupling. So far, the only known three-dimensional topological insulator is Bix Sb1-x , which is an alloy with complex surface states. Here, we present the results of first-principles electronic structure calculations of the layered, stoichiometric crystals Sb2 Te3 , Sb2 Se3 , Bi2 Te3 and Bi2 Se3 . Our calculations predict that Sb2 Te3 , Bi2 Te3 and Bi2 Se3 are topological insulators, whereas Sb2 Se3 is not. These topological insulators have robust and simple surface states consisting of a single Dirac cone at the point. In addition, we predict that Bi2 Se3 has a topologically non-trivial energy gap of 0.3 eV, which is larger than the energy scale of room temperature. We further present a simple and unified continuum model that captures the salient topological features of this class of materials.

ecently, the subject of time-reversal-invariant topological insulators has attracted great attention in condensed-matter physics112 . Topological insulators in two or three dimensions have insulating energy gaps in the bulk, and gapless edge or surface states on the sample boundary that are protected by time-reversal symmetry. The surface states of a three-dimensional (3D) topological insulator consist of an odd number of massless Dirac cones, with a single Dirac cone being the simplest case. The existence of an odd number of massless Dirac cones on the surface is ensured by the Z2 topological invariant79 of the bulk. Furthermore, owing to the Kramers theorem, no time-reversalinvariant perturbation can open up an insulating gap at the Dirac point on the surface. However, a topological insulator can become fully insulating both in the bulk and on the surface if a timereversal-breaking perturbation is introduced on the surface. In this case, the electromagnetic response of three-dimensional (3D) topological insulators is described by the topological term of the form S = ( /2)(/2) d 3 x dt E · B, where E and B are the conventional electromagnetic fields and is the fine-structure constant10 . = 0 describes a conventional insulator, whereas = describes topological insulators. Such a physically measurable and topologically non-trivial response originates from the odd number of Dirac fermions on the surface of a topological insulator. Soon after the theoretical prediction5 , the 2D topological insulator exhibiting the quantum spin Hall effect was experimentally observed in HgTe quantum wells6 . The electronic states of the 2D HgTe quantum wells are well described by a 2 + 1-dimensional Dirac equation where the mass term is continuously tunable by the thickness of the quantum well. Beyond a critical thickness, the Dirac mass term of the 2D quantum well changes sign from being positive to negative, and a pair of gapless helical edge states appears inside the bulk energy gap. This microscopic mechanism for obtaining topological insulators by inverting the bulk Dirac gap spectrum can also be generalized to other 2D and 3D systems. The guiding principle is to search for insulators where the

R

a

z y x

b

A site B site C site

y x

Quintuple layer

c

C A

Se1' Se1 Bi1 Se2 Bi1' Se1' Se1

t1

t2

t3 Bi Se1 Se2

B C A B C

Figure 1 | Crystal structure. a, Crystal structure of Bi2 Se3 with three primitive lattice vectors denoted as t1,2,3 . A quintuple layer with Se1Bi1Se2Bi1 Se1 is indicated by the red square. b, Top view along the z-direction. The triangle lattice in one quintuple layer has three different positions, denoted as A, B and C. c, Side view of the quintuple layer structure. Along the z-direction, the stacking order of Se and Bi atomic layers is ···C(Se1 )A(Se1)B(Bi1)C(Se2)A(Bi1 )B(Se1 )C(Se1)···. The Se1 (Bi1) layer can be related to the Se1 (Bi1 ) layer by an inversion operation in which the Se2 atoms have the role of inversion centres.

conduction and the valence bands have the opposite parity, and a `band inversion' occurs when the strength of some parameter, say the spinorbit coupling (SOC), is tuned. For systems with inversion symmetry, a method based on the parity eigenvalues of band states at time-reversal-invariant points can be applied13 . On the basis of this analysis, the Bix Sb1-x alloy has been predicted

1 Beijing

National Laboratory for Condensed Matter Physics, and Institute of Physics, Chinese Academy of Sciences, Beijing 100190, China, 2 Center for Advanced Study, Tsinghua University, Beijing 100084, China, 3 Department of Physics, McCullough Building, Stanford University, Stanford, California 94305-4045, USA. *e-mail: [email protected]

438

NATURE PHYSICS | VOL 5 | JUNE 2009 | www.nature.com/naturephysics © 2009 Macmillan Publishers Limited. All rights reserved.

NATURE PHYSICS DOI: 10.1038/NPHYS1270

a

2

ARTICLES

b

2

1

1

Energy (eV)

Energy (eV)

0

0

¬1

¬1

¬2

Z

F

L

¬2

Z

F

L

c

K M

d

Sb2Se3 Z K L F Sb2Te 3 Bi2Se3 Bi2Te 3

Figure 2 | Band structure, Brillouin zone and parity eigenvalues. a,b, Band structure for Bi2 Se3 without (a) and with (b) SOC. The dashed line indicates the Fermi level. c, Brillouin zone for Bi2 Se3 with space group R3m. The four inequivalent time-reversal-invariant points are (0,0,0), L(,0,0), F(,,0) and Z(,,). The blue hexagon shows the 2D Brillouin zone of the projected (1, 1, 1) surface, in which the high-symmetry k points , K and M are labelled. d, The parity of the band at the point for the four materials Sb2 Te3 , Sb2 Se3 , Bi2 Se3 and Bi2 Te3 . Here, we show the parities of fourteen occupied bands, including five s bands and nine p bands, and the lowest unoccupied band. The product of the parities for the fourteen occupied bands is given in brackets on the right of each row.

to be a topological insulator for a small range of x, and recently, surface states with an odd number of crossings at the Fermi energy have been observed in angle-resolved photoemission spectroscopy (ARPES) experiments12 . As Bix Sb1-x is an alloy with random substitutional disorder, its electronic structures and dispersion relations are only defined within the mean field, or the coherent potential approximation. Its surface states are also extremely complex, with as many as five or possibly more dispersion branches, which are not easily describable by simple theoretical models. Alloys also tend to have impurity bands inside the nominal bulk energy gap, which could overlap with the surface states. Given the importance of topological insulators as new states of quantum matter, it is important to search for material systems that are stoichiometric crystals with well-defined electronic structures, preferably with simple surface states, and describable by simple theoretical models. Here, we focus on layered, stoichiometric crystals Sb2 Te3 , Sb2 Se3 , Bi2 Te3 and Bi2 Se3 . Our theoretical calculations predict that Sb2 Te3 , Bi2 Te3 and Bi2 Se3 are topological insulators, whereas Sb2 Se3 is not. Most importantly, our theory predicts that Bi2 Se3 has a topologically non-trivial energy gap of 0.3 eV, larger than the energy scale of room temperature. The topological surface states for these crystals are extremely simple, described by a single gapless Dirac cone at the k = 0 point in the surface Brilloiun zone. We also propose a simple and unified continuum model that captures the salient topological features of this class of materials. In this

NATURE PHYSICS | VOL 5 | JUNE 2009 | www.nature.com/naturephysics

precise sense, this class of 3D topological insulators shares the great simplicity of the 2D topological insulators realized in the HgTe quantum wells.

Band structure and parity analysis

Bi2 Se3 , Bi2 Te3 , Sb2 Te3 and Sb2 Se3 share the same rhombohedral ¯ crystal structure with the space group D5 (R3m) with five atoms 3d in one unit cell. We take Bi2 Se3 as an example and show its crystal structure in Fig. 1a, which has layered structures with a triangle lattice within one layer. It has a trigonal axis (three-fold rotation symmetry), defined as the z axis, a binary axis (two-fold rotation symmetry), defined as the x axis, and a bisectrix axis (in the reflection plane), defined as the y axis. The material consists of five-atom layers arranged along the z-direction, known as quintuple layers. Each quintuple layer consists of five atoms with two equivalent Se atoms (denoted as Se1 and Se1 in Fig. 1c), two equivalent Bi atoms (denoted as Bi1 and Bi1 in Fig. 1c) and a third Se atom (denoted as Se2 in Fig. 1c). The coupling is strong between two atomic layers within one quintuple layer but much weaker, predominantly of the van der Waals type, between two quintuple layers. The primitive lattice vectors t1,2,3 and rhombohedral unit cells are shown in Fig. 1a. The Se2 site has the role of an inversion centre and under an inversion operation, Bi1 is changed to Bi1 and Se1 is changed to Se1 . The existence of inversion symmetry enables us to construct eigenstates with definite parity for this system.

439

© 2009 Macmillan Publishers Limited. All rights reserved.

ARTICLES

a

¬ P1x,y,z + + P1x+iy,, P1x¬iy,

NATURE PHYSICS DOI: 10.1038/NPHYS1270

b

0.1

P1+ x,y

+ + P1x+iy,, P1x¬iy,

+ P1x,y,z

Bi

+ P1z

P2¬ ,P2¬ z, z, E (eV)

¬0.1

+ P1z

Se

¬ P2x,y,z

¬ P2z

+ P1z,, P1+ z,

¬ P2z

¬0.3

¬ P2x+iy,, P2¬ x¬iy,

P2+ x,y,z

P2¬ x,y

¬ P0x,y,z

¬ P2¬ , P2x¬iy, x+iy,

¬0.5 0

xc

0.2

0.4 x

0.6

0.8

1.0

(I)

(II)

(III)

Figure 3 | Band sequence. a, Schematic diagram of the evolution from the atomic px,y,z orbitals of Bi and Se into the conduction and valence bands of Bi2 Se3 at the point. The three different stages (I), (II) and (III) represent the effect of turning on chemical bonding, crystal-field splitting and SOC, respectively (see text). The blue dashed line represents the Fermi energy. b, The energy levels |P1+ and |P2- of Bi2 Se3 at the point versus an artificially z z rescaled atomic SOC (Bi) = x0 (Bi) = 1.25x eV,(Se) = x0 (Se) = 0.22x eV (see text). A level crossing occurs between these two states at x = xc 0.6.

Ab initio calculations for Sb2 Te3 , Sb2 Se3 , Bi2 Te3 and Bi2 Se3 are carried out in the framework of the PerdewBurkeErnzerhoftype14 generalized gradient approximation of the density functional theory. The BSTATE package15 with the plane-wave pseudopotential method is used with a k-point grid taken as 10 × 10 × 10 and the kinetic energy cutoff fixed to 340 eV. For Sb2 Te3 , Bi2 Te3 and Bi2 Se3 , the lattice constants are chosen from experiments, whereas for Sb2 Se3 , the lattice parameters are optimized in the self-consistent calculation for rhombohedral crystal structure (a = 4.076 Å, c = 29.830 Å), owing to the lack of experimental data. Our results are consistent with the previous calculations16,17 . In particular, we note that Bi2 Se3 has an energy gap of about 0.3 eV, which agrees well with the experimental data (about 0.20.3 eV; refs 18, 19). In the following, we take the band structure of Bi2 Se3 as an example. Figure 2a and b show the band structure of Bi2 Se3 without and with SOC, respectively. By comparing the two figure parts, one can see clearly that the only qualitative change induced by turning on SOC is an anti-crossing feature around the point, which thus indicates an inversion between the conduction band and valence band due to SOC effects, suggesting that Bi2 Se3 is a topological insulator. To firmly establish the topological nature of this material, we follow the method proposed by Fu and Kane13 . Thus, we calculate the product of the parities of the Bloch wavefunction for the occupied bands at all time-reversal-invariant momenta ,F ,L,Z in the Brillouin zone. As expected, we find that at the point, the parity of one occupied band is changed on turning on SOC, whereas the parity remains unchanged for all occupied bands at the other momenta F ,L,Z . As the system without SOC is guaranteed to be a trivial insulator, we conclude that Bi2 Se3 is a strong topological insulator. The same calculation is carried out for the other three materials, from which we find that Sb2 Te3 and Bi2 Te3 are also strong topological insulators, and Sb2 Se3 is a trivial insulator. The parity eigenvalues of the highest 14 bands below the Fermi level and the first conduction band at the point are listed in Fig. 2d. From this table we can see that the product of parities of occupied bands at the point changes from the trivial material Sb2 Se3 to the three non-trivial materials, owing to an exchange of the highest occupied state and the lowest unoccupied state. This agrees with our earlier analysis that an inversion between the conduction band and valence band occurs at the point. To get a better understanding of the inversion and the parity exchange, we start from the atomic energy levels and consider the effect of crystal-field splitting and SOC on the energy eigenvalues

440

at the point. This is summarized schematically in three stages (I), (II) and (III) in Fig. 3a. As the states near the Fermi surface are mainly coming from p orbitals, we will neglect the effect of s orbitals and start from the atomic p orbitals of Bi (6s2 6p3 ) and Se (4s2 4p4 ). In stage (I), we consider the chemical bonding between Bi and Se atoms within a quintuple layer, which is the largest energy scale in the current problem. First we can recombine the orbitals in a single unit cell according to their parity, which results in three states (two odd, one even) from each Se p orbital and two states (one odd, one even) from each Bi p orbital. The formation of chemical bonding hybridizes the states on Bi and Se atoms, thus pushing down all of the Se states and lifting up all of the Bi states. In Fig. 3a, these five hybridized states are labelled as |P1± , |P2± x,y,z x,y,z and |P0- , where the superscripts +,- stand for the parity of x,y,z the corresponding states. In stage (II), we consider the effect of the crystal-field splitting between different p orbitals. According to the point-group symmetry, the pz orbital is split from the px and py orbitals whereas the last two remain degenerate. After this splitting, the energy levels closest to the Fermi energy turn out to be the pz levels |P1+ and |P2- . In the last stage (III), we take z z into account the effect of SOC. The atomic SOC Hamiltonian is given by Hso = l · S, with l,S being the orbital and spin angular momentum, and is the SOC parameter. The SOC Hamiltonian mixes spin and orbital angular momenta while preserving the total angular momentum, which thus leads to a level repulsion between |P1+ , and |P1+ , , and similar combinations. Consequently, x+iy z the |P1+ , () state is pushed down by the SOC effect and the z |P2- , () state is pushed up. If the SOC is large enough ( > c ), z the order of these two levels is reversed. To see this inversion process explicitly, we also calculate the energy levels |P1+ and |P2- for z z a model Hamiltonian of Bi2 Se3 with artificially rescaled atomic SOC parameters (Bi) = x0 (Bi), (Se) = x0 (Se), as shown in Fig. 3b. Here, 0 (Bi) = 1.25 eV and 0 (Se) = 0.22 eV are the realistic values of Bi and Se atomic SOC parameters, respectively20 . From Fig. 3b, one can see clearly that a level crossing occurs between |P1+ z and |P2- when the SOC is about 60% of the realistic value. As z these two levels have opposite parity, the inversion between them drives the system into a topological insulator phase. Therefore, the mechanism for the 3D topological insulator in this system is exactly analogous to the mechanism in the 2D topological insulator HgTe. In summary, through the analysis above we find that Bi2 Se3 is topologically non-trivial due to the inversion between two pz orbitals with opposite parity at the point. Similar analyses can

NATURE PHYSICS | VOL 5 | JUNE 2009 | www.nature.com/naturephysics © 2009 Macmillan Publishers Limited. All rights reserved.

NATURE PHYSICS DOI: 10.1038/NPHYS1270

a

0.15 0.10 Sb2Se3 8 6 4 2 0 ¬0.05 ¬0.10 ¬0.15 K M 0 ¬2 ¬4 ¬6 ¬8

ARTICLES

b

0.4 0.3 0.2 Sb2Te 3 8 6 4 2 0 ¬2 ¬4 Bi2Te 3 M ¬6 8 6 4 0 ¬0.1 ¬0.2 ¬0.3 K M 2 0 ¬2 ¬4

Energy (eV)

Energy (eV)

0.05

0.1 0 ¬0.1 ¬0.2 K

c

0.4 0.3 0.2 Bi2Se3

8 6 4 2 0 ¬2 ¬4 M ¬6

d

0.2 0.1

Energy (eV)

0.1 0 ¬0.1 ¬0.2 ¬0.3 K

Figure 4 | Surface states. ad, Energy and momentum dependence of the LDOS for Sb2 Se3 (a), Sb2 Te3 (b), Bi2 Se3 (c) and Bi2 Te3 (d) on the [111] surface. Here, the warmer colours represent higher LDOS. The red regions indicate bulk energy bands and the blue regions indicate bulk energy gaps. The surface states can be clearly seen around the point as red lines dispersing in the bulk gap for Sb2 Te3 , Bi2 Se3 and Bi2 Te3 . No surface state exists for Sb2 Se3 .

be carried out on the other three materials, from which we see that Sb2 Te3 and Bi2 Te3 are qualitatively the same as Bi2 Se3 , whereas the SOC of Sb2 Te3 is not strong enough to induce such an inversion.

Topological surface states

The existence of topological surface states is one of the most important properties of the topological insulators. To see the topological features of the four systems explicitly, we calculate the surface states of these four systems on the basis of an ab initio calculation. First we construct the maximally localized Wannier function (MLWF) from the ab initio calculation using the method developed by Marzari and co-workers21,22 . We divide the semiinfinite system into a surface slab with finite thickness and the remaining part as the bulk. The MLWF hopping parameters for the bulk part can be constructed from the bulk ab initio calculation, and the ones for the surface slab can be constructed from the ab initio calculation of the slab, in which the surface correction to the lattice constants and band structure have been considered self-consistently and the chemical potential is determined by the charge neutrality condition. With these bulk and surface MLWF hopping parameters, we use an iterative method23,24 to obtain the surface Green's function of the semi-infinite system. The imaginary part of the surface Green's function is the local density of states (LDOS), from which we can obtain the dispersion of the surface states. The surface LDOS on the [111] surface for all four systems is shown in Fig. 4. For Sb2 Te3 , Bi2 Se3 and Bi2 Te3 , one can clearly see the topological surface states that form a single Dirac cone at the point. In comparison, Sb2 Se3 has no surface state and is a topologically trivial insulator. Thus, the surface-state calculation agrees well with the bulk parity analysis, and confirms conclusively the topologically non-trivial nature of the three materials. For Bi2 Se3 , the Fermi velocity of the topological surface states is vF 5.0 × 105 m s-1 , which is similar to that of the other two materials.

to characterize the low-energy long-wavelength properties of the system. Starting from the four low-lying states |P1+ , () z and |P2- , () at the point, such a Hamiltonian can be z constructed by the theory of invariants25 for the finite wave vector k. On the basis of the symmetries of the system, the generic form of the 4 × 4 effective Hamiltonian can be written down up to the order of O(k2 ), and the tunable parameters in the Hamiltonian can be obtained by fitting the band structure of our ab initio calculation. The important symmetries of the system are time-reversal symmetry T , inversion symmetry I and three-fold rotation symmetry C3 along the z axis. In the basis of (|P1+ , , |P2- , , |P1+ , , |P2- , ), the representation of the z z z z symmetry operations is given by T = K · i y I2×2 , I = I2×2 3 z and C3 = exp(i(/3) I2×2 ), where K is the complex conjugation operator, x,y,z and x,y,z denote the Pauli matrices in the spin and orbital space, respectively. By requiring these three symmetries and keeping only the terms up to quadratic order in k, we obtain the following generic form of the effective Hamiltonian:

M(k) A1 kz H (k) = 0 (k)I4×4 + 0 A2 k+

Energy (eV)

A1 kz -M(k) A2 k+ 0

0 A2 k- M(k) -A1 kz

A2 k- 0 -A1 kz -M(k) (1)

+ o(k2 )

Low-energy effective model

As the topological nature is determined by the physics near the point, it is possible to write down a simple effective Hamiltonian

NATURE PHYSICS | VOL 5 | JUNE 2009 | www.nature.com/naturephysics

2 with k± = kx ± iky , 0 (k) = C + D1 kz2 + D2 k and M(k) = M - B1 2 kz2 - B2 k . By fitting the energy spectrum of the effective Hamiltonian with that of the ab initio calculation, the parameters in the effective model can be determined. For Bi2 Se3 , our fitting 2 leads to M = 0.28 eV, A1 = 2.2 eV Å, A2 = 4.1 eV Å, B1 = 10 eV Å , 2 2 2 B2 = 56.6 eV Å , C = -0.0068 eV, D1 = 1.3 eV Å , D2 = 19.6 eV Å . Except for the identity term 0 (k), the Hamiltonian (1) is nothing but the 3D Dirac model with uniaxial anisotropy along the z-direction and k-dependent mass terms. From the fact

441

© 2009 Macmillan Publishers Limited. All rights reserved.

ARTICLES

M ,B1 ,B2 > 0, we can see that the order of the bands |T 1+ , () z and |T 2- , () is inverted around k = 0 compared with large k, z which correctly characterizes the topologically non-trivial nature of the system. Such an effective Dirac model can be used for further theoretical study of the Bi2 Se3 system, as long as the low-energy properties are considered. For example, as one of the most important low-energy properties of the topological insulators, the topological surface states can be obtained from diagonalizing the effective Hamiltonian equation (1) with an open boundary condition, with the same method used in the study of the 2D quantum spin Hall insulator26 . For a surface perpendicular to the z-direction (that is, the [111] direction), kx , ky are still good quantum numbers but kz is not. By substituting -iz for kz in equation (1), one can write down the 1D Schrödinger equations for the wavefunctions kx ,ky (z). For kx = ky = 0, there are two renormalizable surface-state solutions on the half infinite space z > 0, denoted by |0 , |0 . By projecting the bulk Hamiltonian (1) onto the subspace of these two surface states, to the leading order of kx ,ky we obtain the following surface Hamiltonian Hsurf (kx ,ky ) = 0 A2 k+ A2 k- 0 (2)

NATURE PHYSICS DOI: 10.1038/NPHYS1270

4. Murakami, S. Quantum spin hall effect and enhanced magnetic response by spinorbit coupling. Phys. Rev. Lett. 97, 236805 (2006). 5. Bernevig, B. A., Hughes, T. L. & Zhang, S. C. Quantum spin hall effect and topological phase transition in HgTe quantum wells. Science 314, 17571761 (2006). 6. König, M. et al. Quantum spin hall insulator state in HgTe quantum wells. Science 318, 766770 (2007). 7. Fu, L., Kane, C. L. & Mele, E. J. Topological insulators in three dimensions. Phys. Rev. Lett. 98, 106803 (2007). 8. Moore, J. E. & Balents, L. Topological invariants of time-reversal-invariant band structures. Phys. Rev. B 75, 121306 (2007). 9. Roy, R. On the Z2 classification of quantum spin hall models. Preprint at <http://arxiv.org/abs/cond-mat/0604211> (2006). 10. Qi, X.-L., Hughes, T. L. & Zhang, S.-C. Topological field theory of time-reversal invariant insulators. Phys. Rev. B 78, 195424 (2008). 11. Dai, X., Hughes, T. L., Qi, X.-L., Fang, Z. & Zhang, S.-C. Helical edge and surface states in HgTe quantum wells and bulk insulators. Phys. Rev. B 77, 125319 (2008). 12. Hsieh, D. et al. A topological dirac insulator in a quantum spin hall phase. Nature 452, 970974 (2008). 13. Fu, L. & Kane, C. L. Topological insulators with inversion symmetry. Phys. Rev. B 76, 045302 (2007). 14. Perdew, J. P., Burke, K. & Ernzerhof, M. Generalized gradient approximation made simple. Phys. Rev. Lett. 77, 38653868 (1996). 15. Fang, Z. & Terakura, K. Structural distortion and magnetism in transition metal oxides: Crucial roles of orbital degrees of freedom. J. Phys. Condens. Matter 14, 30013014 (2002). 16. Mishra, S. K., Satpathy, S. & Jepsen, O. Electronic structure and thermoelectric properties of bismuth telluride and bismuth selenide. J. Phys. Condens. Matter 9, 461470 (1997). 17. Larson, P. Effects of uniaxial and hydrostatic pressure on the valence band maximum in Sb2 Te3 : An electronic structure study. Phys. Rev. B 74, 205113 (2006). 18. Black, J., Conwell, E. M., Seigle, L. & Spencer, C. W. Electrical and optical properties of some M2-N3-semiconductors. J. Phys. Chem. Solids 2, 240251 (1957). 19. Mooser, E. & Pearson, W. B. New semiconducting compounds. Phys. Rev. 101, 492493 (1956). 20. Wittel, K. & Manne, R. Atomic spinorbit interaction parameters from spectral data for 19 elements. Theor. Chim. Acta 33, 347349 (1974). 21. Marzari, N. & Vanderbilt, D. Maximally localized generalized wannier functions for composite energy bands. Phys. Rev. B 56, 1284712865 (1997). 22. Souza, I., Marzari, N. & Vanderbilt, D. Maximally localized wannier functions for entangled energy bands. Phys. Rev. B 65, 035109 (2001). 23. Sancho, M. P. L., Sancho, J. M. L. & Rubio, J. Quick iterative scheme for the calculation of transfer matrices: Application to Mo (100). J. Phys. F 14, 12051215 (1984). 24. Sancho, M. P. L., Sancho, J. M. L., Sancho, J. M. L. & Rubio, J. Highly convergent schemes for the calculation of bulk and surface green functions. J. Phys. F 15, 851858 (1985). 25. Winkler, R. SpinOrbit Coupling Effects in Two-Dimensional Electron and Hole Systems (Springer Tracts in Modern Physics, Vol. 191, Springer, 2003). 26. Koenig, M. et al. The quantum spin hall effect: Theory and experiment. J. Phys. Soc. Japan 77, 031007 (2008). 27. Noh, H.-J. et al. Spinorbit interaction effect in the electronic structure of Bi2 Te3 observed by angle-resolved photoemission spectroscopy. Europhys. Lett. 81, 57006 (2008). 28. Urazhdin, S. et al. Surface effects in layered semiconductors Bi2 Se3 and Bi2 Te3 . Phys. Rev. B 69, 085313 (2004). 29. Xia, Y. et al. Electrons on the surface of Bi2 Se3 form a topologically-ordered two dimensional gas with a non-trivial berry's phase. Preprint at <http://arxiv.org/abs/0812.2078> (2008). 30. Qi, X.-L., Li, R.-D., Zang, J. & Zhang, S.-C. Inducing a magnetic monopole with topological surface states. Science 323, 11841187 (2009).

in the basis of |0 ,|0 . Here, the surface-state wavefunction |0() is a superposition of the |P1+ , () and |P2+ , () states, z z respectively. For A2 = 4.1 eV Å obtained from the fitting, the Fermi velocity of the surface states is given by vF = A2 / 6.2×105 m s-1 , which agrees reasonably well with the ab initio results shown in Fig. 4c. In summary, the effective model of the surface states equation (2) characterizes the key features of the topological surface states, and can be used in the future to study the surface-state properties of the Bi2 Se3 family of topological insulators. The topological surface states can be directly verified by various experimental techniques, such as ARPES and scanning tunnelling microscopy. In recent years, evidence of surface states has been observed for Bi2 Se3 and Bi2 Te3 in ARPES (ref. 27) and scanning tunnelling microscopy28 experiments. In particular, the surface states of Bi2 Te3 observed in ref. 27 had a similar dispersion to what we obtained in Fig. 4d, which were also shown to be quite stable and robust, regardless of photon exposure and temperature. Near the completion of this work, we became aware of the ARPES experiment29 on Bi2 Se3 , which measures a Dirac cone near the point of the surface Brilloiun zone. These experimental results support the main conclusion of our theoretical work. Moreover, the 3D topological insulators are predicted to exhibit the universal topological magneto-electric effect10 when the surface is coated with a thin magnetic film. Compared with the Bi1-x Sbx alloy, the surface states of the Bi2 Se3 family of topological insulators contain only a single Fermi pocket, making it easier to open up a gap on the surface by magnetization and to observe the topological Faraday/Kerr rotation10 and image magnetic monopole effect30 . If observed, such effects would be an unambiguous experimental signature of the non-trivial topology of the electronic properties.

Received 8 December 2008; accepted 1 April 2009; published online 10 May 2009

Acknowledgements

We would like to thank B. F. Zhu for the helpful discussion. This work is supported by the NSF of China, the National Basic Research Program of China (No. 2007CB925000), the International Science and Technology Cooperation Program of China (No. 2008DFB00170) and by the US Department of Energy, Office of Basic Energy Sciences under contract DE-AC02-76SF00515.

References

1. Kane, C. L. & Mele, E. J. Quantum spin hall effect in graphene. Phys. Rev. Lett. 95, 226801 (2005). 2. Bernevig, B. A. & Zhang, S. C. Quantum spin hall effect. Phys. Rev. Lett. 96, 106802 (2006). 3. Kane, C. L. & Mele, E. J. Z2 topological order and the quantum spin hall effect. Phys. Rev. Lett. 95, 146802 (2005).

Additional information

Reprints and permissions information is available online at http://npg.nature.com/ reprintsandpermissions. Correspondence and requests for materials should be addressed to S.-C.Z.

442

NATURE PHYSICS | VOL 5 | JUNE 2009 | www.nature.com/naturephysics © 2009 Macmillan Publishers Limited. All rights reserved.

#### Information

##### Topological insulators in Bi2Se3, Bi2Te3 and Sb2Te3 with a single Dirac cone on the surface

5 pages

#### Report File (DMCA)

Our content is added by our users. **We aim to remove reported files within 1 working day.** Please use this link to notify us:

Report this file as copyright or inappropriate

116803

### You might also be interested in

^{BETA}